1 Materials 2014, 7, ; doi: /ma Article OPEN ACCESS materials ISSN Transformation-Induced Relaxation and Stress Recovery of TiNi Shape Memory Alloy Kohei Takeda 1, *, Ryosuke Matsui 1, Hisaaki Tobushi 1 and Elzbieta A. Pieczyska Department of Mechanical Engineering, Aichi Institute of Technology, 1247 Yachigusa, Yakusa-cho, Toyota , Japan; s: (R.M.); (H.T.) Institute of Fundamental Technological Research, Polish Academy of Sciences, Pawinskiego 5B, Warszawa , Poland; * Author to whom correspondence should be addressed; Tel.: ; Fax: Received: 4 December 2013; in revised form: 15 January 2014 / Accepted: 24 February 2014 / Published: 6 March 2014 Abstract: The transformation-induced stress relaxation and stress recovery of TiNi shape memory alloy (SMA) in stress-controlled subloop loading were investigated based on the local variation in temperature and transformation band on the surface of the tape in the tension test. The results obtained are summarized as follows. (1) In the loading process, temperature increases due to the exothermic martensitic transformation (MT) until the holding strain and thereafter temperature decreases while holding the strain constant, resulting in stress relaxation due to the MT; (2) In the unloading process, temperature decreases due to the endothermic reverse transformation until the holding strain and thereafter temperature increases while holding the strain constant, resulting in stress recovery due to the reverse transformation; (3) Stress varies markedly in the initial stage followed by gradual change while holding the strain constant; (4) If the stress rate is high until the holding strain in the loading and unloading processes, both stress relaxation and stress recovery are large; (5) It is important to take into account this behavior in the design of SMA elements, since the force of SMA elements varies even if the atmospheric temperature is kept constant. Keywords: shape memory alloy; superelasticity; titanium-nickel alloy; subloop; stress relaxation; stress recovery; martensitic transformation
2 Materials 2014, Introduction Since shape memory alloy (SMA) shows shape memory effect and superelasticity (SE) and has superior functions as an intelligent material, the application of the SMA has drawn worldwide attention [1 3]. In order to design shape memory elements in the application of SMA, the thermomechanical properties of the material are important. The functional properties of SMA appear mainly based on the martensitic transformation (MT). Since the MT of the SMA depends on temperature, stress and their hysteresis, the deformation properties due to the MT are complex [4 6]. Most studies on the thermomechanical properties have been carried out until now under the condition of a full or perfect loop in which the MT and reverse transformation complete. In practical applications, strain, temperature and stress vary in various ranges. In the case of the subloop, partial loop, or inner loop in which strain, temperature, and stress vary in the range prior to the MT completion, the starting and finishing conditions of the MT prescribed in the full loop are not satisfied. The progress of the MT and reverse transformation therefore changes depending on the hysteresis of strain, temperature and stress [7 9]. For example, two-way deformation appears in the SMA element due to the MT and reverse transformation by heating and cooling under constant stress. In the case of the full loop, the SMA element elongates and shrinks by the amount of deformation or stroke corresponding to the available MT strain. However, in the case of subloop, the stroke corresponding to the MT strain cannot be obtained in the SMA element. In a similar way, since the recovery stress which appears by heating and cooling under constant strain varies depending on the hysteresis, the recovery stress in the subloop becomes smaller than that in the full loop. Therefore, when the recovery stress is used as the driving force of actuator or robot, the recovery stress in the subloop cannot be used effectively, as in the full loop. In addition, since the MT depends on the rates of loading-unloading and heating-cooling, the variations in strain and stress are complex. If the SMA is subjected to subloop loading, the transformation-induced creep appears under constant stress  and the transformation-induced stress relaxation occurs under constant strain . In this paper, although variation in stress was considered to be induced due to either an exothermic or endothermic reaction, the variation in temperature distribution on the specimen surface was not observed directly. It has not been observed up to the present since the amount of progress of the MT is small under constant strain and therefore the observation of the transformation progressing process is not easy. In practical applications of SMA like in a clutch or a brake to control the motion of machines, in an actuator to control the driving force by oil pressure and in a tightening element, it is necessary to control the load. If SMA is used in these devices, it is necessary to understand the deformation behavior in the stress-controlled condition. In many cases of these SMA applications, the element is controlled to operate in a certain position and thereafter to keep the position. If the condition of the MT to progress is satisfied, stress relaxation and stress recovery occur under constant strain and the load to hold the position varies. Similarly, even if the load is controlled to remain constant in order to hold the position, creep and creep recovery may occur under constant stress, resulting in difficulty in controlling the position. Therefore, considering the control of load and position by using the SMA, it is necessary to understand the stress-strain-temperature relationship of the SMA. In order to evaluate the functional properties of SMA elements subjected to subloop loading and to design the SMA elements for practical use, the deformation behavior in the subloop loading is very important.
3 Materials 2014, In the present study, transformation-induced relaxation and stress recovery in the stress-controlled SE subloop loading are discussed with a tension test for TiNi SMA, which is most widely used in practical applications. If it is loaded under a constant stress rate and thereafter strain is held constant in the MT region, stress relaxation appears. If strain is held constant in the reverse transformation region during unloading, stress recovery appears. Although phase transformation front propagation has been investigated in full loop loading under a constant strain rate or stress rate [11,12], phase transformation front propagation has been reported little in subloop loading. In particular, since front propagation under a constant strain is very small and not easy to observe, it has not been reported up until now. Based on the changes in the transformation band observed by microscope and the temperature distribution by thermography on the specimen surface in the experiment, the characteristics of stress relaxation and stress recovery have been clarified. The influence of stress rate on the stress relaxation and stress recovery is also discussed. 2. Deformation Properties in Subloop Strain-Controlled and Stress-Controlled Loadings The SE stress-strain diagrams in subloop strain-controlled and stress-controlled loadings under a constant low strain rate, high strain rate and stress rate are schematically shown in Figure 1a c, respectively [9,13]. As shown in Figure 1a, in the case of subloop unloading from a point b and reloading from a point d under a constant low strain rate, the second upper stress plateau during reloading appears due to the MT at a point e under a little lower stress than that in the first stress plateau and thereafter the curve passes through the unloading start point b, showing the return-point memory [5,9,13]. Figure 1. Stress-strain diagrams in superelasticity (SE) subloop strain-controlled and stress-controlled loadings under various loading rates. (a) Constant low strain rate; (b) Constant high strain rate; (c) Constant stress rate. (a) (b) (c)
4 Materials 2014, As shown in Figure 1b, in the case of subloop loading and unloading under a constant high strain rate, temperature increases due to the exothermic stress-induced martensitic transformation (SIMT) and stress increases in the upper stress plateau. If it is reloaded from a point d following unloading from a point b, the SIMT starts at a point e and the reloading curve does not pass through the point b. The return-point memory therefore does not appear. As shown in Figure 1c, in the case of subloop loading and unloading under a constant stress rate, stress increases in the loading process from a point A to a point B since temperature increases due to the SIMT. In the unloading process from the point B, the material is cooled by the air, resulting in a decrease in temperature. The condition for the MT to progress therefore is satisfied in the unloading process from point B to a point C, and strain increases with accompaniment of an overshoot of strain. Temperature decreases due to the reverse transformation in the unloading process from a point D to a point E, and temperature increases due to heating by the air in the reloading process from point E to a point F. The condition for the reverse transformation to progress therefore is satisfied from point E to point F, and strain decreases with accompaniment of an undershoot of strain . The following reloading curve from a point G to a point H in the transformation region does not pass through the unloading start point B and the return-point memory therefore does not appear. As mentioned above, in stress-controlled subloop loading, overshoot and undershoot of strain appear in the early stage of unloading and reloading and do not appear in strain-controlled subloop loading. Therefore, in order to design SMA elements which control force, it is important to understand the deformation behavior in the stress-controlled subloop loading. 3. Experimental Method 3.1. Materials and Specimen The material was a Ti-50.95at%Ni SMA tape to show SE at room temperature, produced by Furukawa Techno Material, Co., Ltd. (Hiratsuka, Japan). Thickness of the material was 0.37 mm, width 9.95 mm and length 170 mm. The material was held at 803 K for 1 min in the shape-memory heat treatment process. The differential scanning calorimetry (DSC) (Shimadzu, Co., Kyoto, Japan) thermogram of the material is shown in Figure 2. The R-phase transformation start and finish temperatures R s and R f, and the reverse transformation start and finish temperatures A s and A f obtained by the DSC were 279 K, 245 K, 247 K and 281 K, respectively. The specimen was the tape with uniform shape. The gauge length was the distance of 100 mm between grippers. The specimen surface to observe the transformation band was mirror-finished with emery paper No The specimen surface to observe the temperature distribution by thermography was covered with a uniform thin soot layer from a candle. In the process of covering the specimen surface with the soot, a small plate was used for the soot formation between the specimen and a candle. With this procedure, the specimen was kept away from the candle flame, and the influence of heat while covering the specimen surface with the soot was therefore slight.
5 Materials 2014, Figure 2. Differential scanning calorimetry (DSC) thermogram for material used in the experiments Experimental Apparatus The SMA-characteristic testing machine (EZ Graph, Shimadzu, Co., Kyoto, Japan) was used in the tension test. The transformation band on the specimen surface was observed by a motion analysis microscope (VW-6000, Keyence, Co., Osaka, Japan). The temperature variation due to the exothermic and endothermic MT on the specimen surface was observed by infrared thermography (Thermo Tracer H2600, Nippon Avionics, Co., Ltd., Tokyo, Japan) Experimental Procedure The tension test on the stress relaxation and stress recovery characteristics in the stress-controlled SE subloop loading was carried out at room temperature in air. The transformation band and temperature distribution on the specimen surface were observed during the test. The loading process took place under a constant stress rate dσ/dt until a certain strain ε 1 and thereafter stress relaxation was observed by holding ε 1 constant. The following unloading process was conducted under a constant stress rate dσ/dt until a certain strain ε 3 and thereafter stress recovery was observed by holding ε 3 constant. The stress rates dσ/dt were 1 MPa/s, 3 MPa/s and 5MPa/s. The holding strains ε 1 and ε 3 in the loading and unloading processes were 6% and 2%, respectively. 4. Experimental Results and Discussion 4.1. Stress relaxation and Stress Recovery Stress-Strain Relationship in Stress-Controlled Subloop Loading The stress-strain curve and variations in stress σ and strain ε with time t obtained by the test under a stress rate dσ/dt = 5 MPa/s until a point H 1 at a strain ε 1 = 6% followed by holding the strain ε 1 constant and thereafter unloading under a stress rate dσ/dt = 5 MPa/s until a point H 3 at a strain ε 3 = 2% followed by holding the strain ε 3 constant, are shown in Figures 3 and 4, respectively.
6 Materials 2014, As can be seen in Figure 3, in the strain holding process at ε 1 = 6% following loading till the strain ε 1 under the stress rate dσ/dt = 5 MPa/s, stress decreases from σ 1 to σ 2, resulting in stress relaxation σ = σ 2 σ 1. In the strain holding process at ε 3 = 2% following unloading till the strain ε 3 under the stress rate dσ/dt = 5 MPa/s, stress increases from σ 3 to σ 4, resulting in stress recovery σ = σ 4 σ 3. Stress fluctuates just after a MT starting point S M in the loading process as observed in Figures 3 and 4. Figure 3. Stress-strain curve obtained by the test under a stress rate of dσ/dt = 5 MPa/s until a point H 1 followed by holding strain constant at ε 1 = 6% and thereafter unloading until a point H 3 followed by holding the strain constant at ε 3 = 2%. Figure 4. Variation in stress and strain with time obtained by the test under a stress rate of dσ/dt = 5 MPa/s until a point H 1 followed by holding the strain constant until a point H 2 and thereafter unloading until a point H 3 followed by holding the strain constant until a point H 4. The transformation band occurs due to the SIMT at the point S M, and an overshoot of stress appears. Compared to a strain rate dε/dt = s 1 until the point S M, the strain rate dε/dt increases suddenly to s 1 after the point S M. This is caused by the fact that a cross-head in the tension test machine moves under higher velocity since it is being controlled to keep a constant stress rate, and
7 Materials 2014, an overshoot of stress therefore appears. In order to follow this sudden velocity change, first of all stress fluctuates just after the point S M. Then after the strain holding start point H 1, stress decreases rapidly in the early stage and thereafter decreases gradually. The stress σ 2 at a point H 2 after relaxation is 397 MPa. Similarly, in the unloading process, since undershoot of stress appears, the strain rate dε/dt increases suddenly from s 1 to s 1 after the reverse transformation start point S A. After the strain holding start point H 3, stress increases rapidly in the early stage and thereafter increases gradually. The stress σ 4 at a point H 4 after recovery is 263 MPa Behavior of the Transformation Band Figure 5 shows the photographs of the specimen surface at various strains taken by a microscope during the test which correspond to the stress-strain curve shown in Figure 3. The photograph on the right hand side shows the surface without tinting at a strain of 4% in the loading process. As can be seen from this photograph, although the interface of the transformation band can be observed, the region of the austenite phase (A-phase) and that of the martensitic phase (M-phase) are not clearly recognized at a glance. In order to show the region of the M-phase clearly, the M-phase is tinted by deep blue in Figure 5. In the loading process under a constant stress rate of 5 MPa/s, strain rate dε/dt increases from a strain of 2% to 3%, and the transformation bands appear on the whole specimen surface. After a strain of 3%, the interfaces of the appeared transformation bands propagate and strain increases. In the strain holding stage from the point H 1 at a strain of 6% to the point H 2, the MT progresses and the region of the M-phase expands a little. In the unloading process after stress relaxation (point H 2 ), the reverse transformation progresses from the initiation location at the interfaces of the transformation bands and strain decreases. In the strain holding stage from the point H 3 at a strain of 2% to the point H 4, the reverse transformation progresses and the region of the A-phase expands a little. Figure 5. Photographs of specimen surface at various strains ε under a stress rate of 5 MPa/s followed by holding strain constant at a point H 1 (ε 1 = 6%) during loading and at a point H 3 (ε 3 = 2%) during unloading.
8 Materials 2014, As mentioned above, it is thus apparent that stress relaxation and stress recovery are due to the transformation progress under constant strain Temperature Change due to Transformation Figure 6 shows the temperature distributions on the specimen surface at various strains during loading and at various stresses while holding the strain constant, obtained by thermography in the test which was carried out under the same conditions as the stress-strain curve shown in Figure 3. Figure 7 shows the relationship of stress σ and temperature change T between the average temperature on the specimen surface and the atmospheric temperature with time t during loading while holding the strain constant. In the same manner, the thermograms of temperature distribution on the specimen surface and the relationship of stress σ and the temperature change T during unloading while holding the strain constant with time t are shown in Figures 8 and 9, respectively. With respect to the thermograms in Figures 6 and 8, in order to express the variation in temperature distribution on the specimen surface while holding the strain constant, the temperature distributions are shown clearly at each stress interval σ = 20 MPa. Figure 6. Thermograms of temperature distribution on the specimen surface at various strains ε during loading under a stress rate of 5 MPa/s until a point H 1 (ε 1 = 6%) and at various stresses σ while holding the strain constant at 6% until point H 2. As can be seen in Figures 6 and 7, in the loading process from the MT start point S M to the point H 1 (ε 1 = 6%) under a constant stress rate dσ/dt = 5 MPa/s, strain rate becomes high as shown in Figure 4 and there exists less time for the heat generated due to the exothermic MT to transfer to the atmospheric air, resulting in an increase in temperature of the specimen. In the strain holding stage from point H 1 to point H 2, the temperature decreases due to the air and the condition for the transformation to progress is satisfied, resulting in progress of the MT. As a result, stress relaxation appears while holding the strain constant.
9 Materials 2014, Figure 7. Variation in stress σ and average temperature change ΔT on the specimen surface with time t during loading under a stress rate of 5 MPa/s until a point H 1 (ε 1 = 6%) and while holding the strain constant at 6% from point H 1 to point H 2. Figure 8. Thermograms of temperature distribution on the specimen surface at various strains ε during unloading under a stress rate of 5 MPa/s till a point H 3 (ε 3 = 2%) and at various stresses σ while holding the strain constant at 2% until point H 4. As can be seen in Figures 8 and 9, in the unloading process from the reverse transformation start point S A to the point H 3 (ε 2 = 2%) under a constant stress rate dσ/dt = 5 MPa/s, the strain rate becomes high and the temperature decreases due to the endothermic reverse transformation. In the following strain holding stage, the temperature increases due to the air and the condition for the transformation to progress is satisfied. As a result, stress recovery appears due to the reverse transformation while holding the strain constant from point H 3 to point H 4. As can be seen in Figures 7 and 9, the temperature varies markedly in the early stage while holding the strain constant and thereafter saturates to a certain value.
10 Materials 2014, As mentioned above, the temperature varies due to the progress of the transformation in the strain holding process. It can be stated that stress relaxation and stress recovery appear to be based on this temperature variation. Figure 9. Variation in stress σ and average temperature change ΔT on the specimen surface with time t during unloading under a stress rate of 5 MPa/s until a point H 3 (ε 3 = 2%) and while holding the strain constant at 2% from point H 3 to point H Condition for Transformation-Induced Stress Relaxation and Stress Recovery to Progress in Stress-Controlled Subloop Loading In Figure 10, the stress-strain diagram in the SE subloop loading: (1) under a low strain rate is shown by a broken line and (2) by a solid line for the stress relaxation and stress recovery under constant stress rate followed by holding the strain constant and thereafter unloading under a constant stress rate followed by holding the strain constant. The stress-temperature paths for stress relaxation and stress recovery in the stress-controlled subloop loading are shown on the stress-temperature phase diagram in Figure 11. The symbols A, B, C, D, E and F in Figure 10 correspond to those in Figure 11, respectively. Figure 10. Stress-strain diagrams under (1) the strain-controlled condition (broken line) and (2) the stress-controlled condition (solid line) in SE subloop loading.
11 Materials 2014, Figure 11. Stress-temperature paths for stress relaxation and stress recovery in the stress-controlled subloop loading (BC and EF: constant strain) on the stress-temperature phase diagram. In Figure 11, z denotes the volume fraction of the M-phase, and z B and z E denote the volume fractions at a point B and a point E, respectively. The symbols M S, M F, A S and A F denote the start and finish lines of the MT and the reverse transformation with the slopes C M and C A, respectively. The broken lines M B and A E express the states at the volume fractions z B and z E, respectively. The conditions for the transformations to progress are expressed by the following equations . dσ/dt C M : for dt > 0 dσ/dt C M : for dt < 0 dσ/dt C A : for dt > 0 dσ/dt C A : for dt < 0 (1) (2) Equation (1) shows the condition for the MT to progress and Equation (2) for the reverse transformation. In the case of a low strain rate, the MT and reverse transformation progress under a constant stress from a to b and from c to d as shown in Figure 10, respectively. In this case, since the strain rate is low and there exists enough time for the heat generated due to the transformation to transfer to the atmosphere, the temperature change of the specimen is slight and both transformations therefore progress under a constant stress. On the other hand, in the case of the stress-controlled loading and unloading, as shown in Figure 11, since strain rate increases from the transformation start points A (S M ) and D (S A ), the temperature of the specimen changes during AB and DE. As a result, if the strain is held constant thereafter, transformation-induced stress relaxation (during BC) and stress recovery (during EF) appear. In the stress relaxation and stress recovery process, stress changes under constant strain. If it is assumed that the strain change ε is composed of the elastic strain change ε e and the transformation strain change ε t, ε = ε e + ε t = 0 while holding the strain constant. If the transformation strain change ε t appears based on temperature change, the elastic strain change ε e = ε t. The relation between elastic strain change ε e and stress change σ is as follows, ε e = σ/e, where E denotes the elastic modulus. Therefore, stress change σ = E ε t. As expressed by this equation, if the transformation progresses under constant strain, the stress varies.
12 Materials 2014, If stress is held constant at point B in Figure 10, transformation-induced creep appears (from point B to point B ). The creep appears due to the MT progress. With respect to the creep deformation, since the MT progresses based on a temperature decrease under constant stress, the strain increases [10,13] Influence of Stress Rate on Stress Relaxation and Stress Recovery The parameters which can be controlled for the thermomechanical properties shown in Figures 10 and 11 are stress rate, holding strain, atmospheric temperature and strain holding time. In the present study, with respect to the constant holding strains ε 1 = 6% during loading and ε 3 = 2% during unloading, the constant atmospheric temperature and the strain holding time for the stress to saturate a certain value, the influence of various stress rates dσ/dt on stress relaxation and stress recovery was investigated. The stress-strain curves obtained by the test are shown in Figure 12. As can be seen in Figure 12, the higher the stress rate dσ/dt in the loading process, then the larger is the temperature rise due to the MT in the upper stress plateau and the higher the stress σ at point H 1. This is caused by the fact that the transformation stress increases in proportion to temperature as shown in Figure 11. On the other hand, the stress σ at the point H 2 does not depend on stress rate and takes almost the same value. As a result, the higher the stress rate, then the larger is the amount of stress relaxation σ from point H 1 to H 2. In the unloading process, the higher the stress rate, then the larger is the decrease in temperature due to the reverse transformation in the lower stress plateau and the lower the stress σ at the point H 3. On the other hand, the stress σ at the point H 4 does not depend on stress rate and takes almost the same value. As a result, the higher the stress rate, the larger is the amount of stress recovery σ. The dependence of the characteristics in stress relaxation and stress recovery on the holding strain, atmospheric temperature, strain holding time and stress is a future subject. Figure 12. Stress-strain curves obtained by the test under various stress rates dσ/dt until point H 1 followed by holding the strain constant at ε 1 = 6% and thereafter unloading until point H 3 followed by holding the strain constant at ε 3 = 2%. As found from the experimental results mentioned above, based on the variation in temperature in the loading and unloading processes, stress relaxation and stress recovery appear due to the progress of the phase transformation under constant strain. Although the change in recovery force of SMA
13 Materials 2014, elements due to the temperature change of the atmospheric medium is used in many applications of SMA, the recovery force of SMA does change without temperature change of the atmospheric medium in the stress-controlled subloop loading, accompanied by temperature change due to an increase in strain rate. This point should be noted in the design of SMA elements. In order to understand the stress relaxation and stress recovery in more detail, it is very important to discuss the deformation properties based on the observation of the microstructure of the material. This subject is for future work. 5. Conclusions The transformation-induced stress relaxation and stress recovery of TiNi SMA tape for SE deformation in stress-controlled subloop loading in the tension test were investigated based on local variation in the transformation band and temperature distribution on the specimen surface observed by microscope and thermography. The influence of the stress rate on stress relaxation and stress recovery is also discussed. The results obtained are summarized as follows. (1) In the loading process under constant stress rate, strain rate increases after the MT starting point and there exists little time for heat generated due to the exothermic MT to transfer to the atmosphere, resulting in temperature rise. In the following strain holding process, the material is cooled by the atmospheric air and the temperature decreases, resulting in stress relaxation due to the MT; (2) In the unloading process under constant stress rate, temperature decreases due to the endothermic reverse transformation after the reverse transformation start point. In the following strain holding process, the material is heated by the atmospheric air and temperature increases, resulting in stress recovery due to the reverse transformation; (3) In the strain holding process, the average temperature on the specimen surface varies markedly in the early stage and thereafter gradually recovers the original temperature. Corresponding to this temperature change, stress relaxation and stress recovery appear markedly in the early stage while holding the strain constant and thereafter stress saturates gradually to a certain value; (4) The behavior of stress relaxation and stress recovery due to the progress of the MT has been confirmed directly by the surface observation of the material; (5) If the stress rate is high until holding the strain constant in the loading and unloading processes, both stress relaxation and stress recovery are large; (6) It is important to take into account stress relaxation and stress recovery in the stress-controlled subloop loading in the design of SMA elements since the force of SMA elements varies due to the temperature variation of the material during loading and unloading even if the atmospheric temperature is kept constant. The fact should be noted that stress relaxation or stress recovery under constant strain occurs without cooling or heating in the SMA elements subjected to the stress-controlled subloop loading.
14 Materials 2014, Acknowledgments The experimental work for the present study was carried out with the assistance of students at Aichi Institute of Technology, to whom the authors wish to express their gratitude. The authors are grateful for the financial support of Grant-in-Aid for Scientific Research (C) No by the Japan Society for Promotion of Science and Grant No. 2011/01/M/ST8/07754 by the Polish National Center of Science. Author Contributions Kohei Takeda: Experiment and discussion; Ryosuke Matsui: Experiment and discussion; Hisaaki Tobushi: Discussion; Elzbieta A. Pieczyska: Discussion. Conflicts of Interest The authors declare no conflict of interest. References 1. Funakubo, H., Ed.; Shape Memory Alloys; Gordon and Breach Science Pub.: New York, NY, USA, 1987; pp Otsuka, K., Wayman, C.M., Eds.; Shape Memory Materials; Cambridge University Press: Cambridge, UK, 1998; pp Miyazaki, S., Ed.; SMST-2007; ASM International: Novelty, Orlando, FL, USA, 2008; pp Tanaka, K.; Kobayashi, S.; Sato, Y. Thermomechanics of Transformation Pseudoelasticity and Shape Memory Effect in Alloys. Int. J. Plast. 1986, 2, Raniecki, B.; Lexcellent, C.; Tanaka, K. Thermodynamic Model of Pseudoelastic Behaviour of Shape Memory Alloys. Arch. Mech. 1992, 44, Tobushi, H.; Matsui, R.; Takeda, K.; Pieczyska, E.A. Mechanical Properties of Shape Memory Materials; Nova Science Pub.: New York, NY, USA, 2013; pp Tanaka, K.; Nishimura, F.; Tobushi, H. Phenomenological Analysis on Subloops in Shape Memory Alloys Due to Incomplete Transformation. J. Intell. Mater. Syst. Struct. 1994, 5, Tanaka, K.; Nishimura, F.; Hayashi, T.; Tobushi, H.; Lexcellent, C. Phenomenological Analysis on Subloop and Cyclic Behavior in Shape Memory Alloys under Mechanical and/or Thermal Loads. Mech. Mater. 1995, 19, Pieczyska, E.A.; Tobushi, H.; Nowacki, W.K.; Gadaj, S.P.; Sakuragi, T. Subloop Deformation Behavior of NiTi Shape Memory Alloy Subjected to Stress-Controlled Loadings. Mater. Trans. 2007, 48, Takeda, K.; Tobushi, H.; Pieczyska, E.A. Transformation-Induced Creep and Creep Recovery of Shape Memory Alloy. Materials 2012, 5, Show, J.A.; Kyriakides, S. Thermomechanical aspects of NiTi. J. Mech. Phys. Solids 1995, 43,
15 Materials 2014, Pieczyska, E.; Gadaj, S.; Nowacki, W.; Tobushi, H. Investigation of Nucleation and Propagation of Phase Transitions in TiNi SMA. Int. J. IR Thermogr. 2004, 1, Takeda, K.; Tobushi, H.; Miyamoto, K.; Pieczyska, E.A. Superelastic Deformation of TiNi Shape Memory Alloy Subjected to Various Subloop Loadings. Mater. Trans. 2012, 53, by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (
A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S Volume 56 2011 Issue 2 DOI: 10.2478/v10172-011-0043-7 E. PIECZYSKA, J. DUTKIEWICZ, F. MASDEU, J. LUCKNER, R. MACIAK INVESTIGATION OF THERMOMECHANICAL
Materials Physics and Mechanics 13 (2012) 64-69 Received: March 13, 2012 CHANGE IN THE TRANSFORMATION SEQUENCE DUE TO STRESS- FREE THERMAL CYCLING OF NI-TI SHAPE MEMORY ALLOY Krzysztof Kuś 1*, Teodor Breczko
Abstract of PhD Thesis Elastic and dissipative energies in phase transformations of Cu-based shape memory alloys Tarek Yousif AbdelRaoof El Rasasi Supervisor Prof. Dezső Beke University of Debrecen PhD
A Study of the Properties of a High Temperature Binary Nitinol Alloy Above and Below its Martensite to Austenite Transformation Temperature Dennis W. Norwich, P.E. SAES Memry Corporation, Bethel, CT Abstract
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
Materials Transactions, Vol. 43, No. 5 (2002) pp. 840 to 845 Special Issue on Smart Materials-Fundamentals and Applications c 2002 The Japan Institute of Metals Hot Water Jet Erosion Characteristics of
We are Nitinol. www.nitinol.com 47533 Westinghouse Drive Fremont, California 94539 t 510.683.2000 f 510.683.2001 Proceedings of the International Conference on Shape Memory and Superelastic Technologies
CHANGES IN THE MECHANICAL BEHAVIOR OF NITINOL FOLLOWING VARIATIONS OF HEAT TREATMENT DURATION AND TEMPERATURE A Thesis Presented to The Academic Faculty By Heidi F. Khalil In Partial Fulfillment Of the
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 2322-5009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277-284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
610 N. Whitney Way, Suite 160 Madison, Wisconsin 53705, USA Phone No: (608) 238-2171 Fax No: (608) 238-9241 email@example.com http://www.powline.com Linear Elastic Cable Model With Creep Proportional to
JOURNAL DE PHYSIQUE IV Colloque C2, supplkment au Journal de Physique 111, Volume 5, fkvrier 1995 Stabilisation of Martensite During Training of CuAlNi Single Crystals C. ~in~fu(l), I. Hurtado, R. Stalmans
EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON
Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi-221
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 28-32 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
The Effects of Varying Active A f Temperatures on the Fatigue Properties of Nitinol Wire M. Patel, D. Plumley, R. Bouthot Fort Wayne Metals Research Products Corporation, Fort Wayne, Indiana, USA J. Proft
MODELING OF CONNECTING STRUCTURE FOR PIPE JOINING WITH APPLICATION TO Fe- Mn-Si SHAPE MEMORY ALLOYS SLEEVES Ion MITELEA a,, Dieter Schinle a, Corneliu Marius Craciunescu a, Ion-Dragos UTU a a POLITEHNICA
Report No. UCB/SEMM-2015/02 Structural Engineering Mechanics and Materials Thermal Phase Transformations in Commercial Dental Files By Rajiv G. Govindjee and Sanjay Govindjee July 2015 Department of Civil
13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 1-6, 24 Paper No. 676 A PERFORMANCE TEST STUDY ON CHINESE G4 LEAD RUBBER BEARINGS Demin FENG 1, Cliff CHEN 2, Wenguang LIU
RESEARCH ARTICLE OPEN ACCESS Life Management Technique of Thermal Fatigue for SMST Boiler Tube at Different Heating Zone Using Smithy Furnace Shekhar Pal, Pradeep Suman, Shri dk jain.gpc kota M-Tech in
Mater. Res. Soc. Symp. Proc. Vol. 855E 2005 Materials Research Society W1.7.1 Applying NiTi Shape-Memory Thin Films to Thermomechanical Data Storage Technology Wendy C. Crone 1, Gordon A. Shaw 2 1 Department
Scripta mater. 44 (2001) 105 110 www.elsevier.com/locate/scriptamat A NOVEL SINTERING-DISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS Y.Y. Zhao and D.X. Sun Materials Science and Engineering, Department
The Mechanical Behavior and Buckling Failure of Sharp-Notched SUS 304 Stainless Steel Tubes Subjected to Pure Bending Creep * Kuo-Long Lee 1) and *Wen-Fung Pan 2) 1) Department of Innovative Design and
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, firstname.lastname@example.org;
FRETTING FATIGUE OF STEELS WITH IFFERENT STRENGTH Václav LINHART, Martin ČIPERA, Dagmar MIKULOVÁ SVÚM, a.s., Podnikatelská 565, 190 11 Praha 9- Běchovice,Czech Republic Abstract The investigation of fretting
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
Product Information Mylar polyester film Physical-Thermal Properties Mylar polyester film retains good physical properties over a wide temperature range ( 7 to 15 C [ 9 to 3 F]), and it is also used at
NANOSYSTEMS: PHYSICS, CHEMISTRY, MATHEMATICS, 2011, 2 (2), P. 76 83 UDC 538.97 MOLECULAR DYNAMICS INVESTIGATION OF DEFORMATION RESPONSE OF THIN-FILM METALLIC NANOSTRUCTURES UNDER HEATING I. S. Konovalenko
CO-MAT-TECH 2005 TRNAVA, 20-21 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK
The Material Properties of Cement Paste with Fly Ash Exposed to High s PAVEL PADEVĚT, ROMANA LOVICHOVÁ Department of Mechanics Czech Technical University in Prague Thákurova 7, 166 29, Prague 6 CZECH REPUBLIC
Infrared Study of Heat Dissipation under Fatigue Crack Propagation O. Plekhov, M. Bannikov, A. erekhina, A. Fedorova Physical foundation of strength Institute of continuous media mechanics RAS str. Ak.
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
A study of cooling process and temperature distribution on a deflating balloon Mei Lingfei Wang Hanwei Tianjin Experimental High School Abstract The surface temperature of a balloon would decrease during
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
http : //www.cigre.org B1-196 AORC Technical meeting 214 Evaluation of Insulating Materials for HVDC Transmission Cable using Space Charge Measurement Y. TANAKA Tokyo City University Japan SUMMARY Some
Proceedings, International Conference on Shape Memory and Superelastic Technologies (SMST-2000), Pacific Grove, California, p.235 (2000) NiTiNb PLUGS FOR SEALING HIGH PRESSURE FUEL PASSAGES IN FUEL INJECTOR
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stress-strain diagram Mild steel : proportional stage, elastic limit, yielding
Comparison of Three Ni-Hard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, Jan-Feb 2016, pp. 119-130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
J. Phys. IVFrance 11 (2001) Pr8487 EDP Sciences, Les Ulis High temperature CuAINb based shape memory alloys J. Lelatko and H. Morawiec Institute of Physics and Chemistry of Metals, University of Silesia,
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, Netphen-Deuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B-306) INTRODUCTION TENSION TEST Mechanical testing
Proceedings of the 12th International Conference on Aluminium Alloys, September 5-9, 2010, Yokohama, Japan 2010 The Japan Institute of Light Metals pp. 1856-1861 1856 Influence of Magnesium on Formation
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
MATEC Web of Conferences 6, 06002 (2013) DOI: 10.1051/matecconf/20130606002 C Owned by the authors, published by EDP Sciences, 2013 Experimental assessment of concrete damage due to exposure to high temperature
Basic Fluid Mechanics MEM 220 Prof. Young I Cho Summer 2009 Chapter 1 Introduction What is fluid? Give some examples of fluids. Examples of gases: Examples of liquids: What is fluid mechanics? Mechanics
EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL Ladislav KANDER a, Miroslav GREGER b a MATERIÁLOVÝ A METALURGICKÝ VÝZKUM, s.r.o., Ostrava, Czech Republic,
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
EUROLAB 25 years The role of metrology and testing to characterize materials and products April 9, 2015, Odense Danmark 1 Origin of Conformity Assessment The New Approach for the European Economic Community
DETERMINATION OF THE HEAT STORAGE CAPACITY OF PCM AND PCM-OBJECTS AS A FUNCTION OF TEMPERATURE E. Günther, S. Hiebler, H. Mehling Bavarian Center for Applied Energy Research (ZAE Bayern) Walther-Meißner-Str.
Theoretical and Practical Aspects of Thermo Mechanical Reliability in Printed Circuit Boards with Copper Plated Through Holes Stefan Neumann, Nina Dambrowsky, Stephen Kenny Atotech Deutschland GmbH Berlin,
Proceedings of the XIth International Congress and Exposition June 2-5, 2008 Orlando, Florida USA 2008 Society for Experimental Mechanics Inc. Effect of Temperature and Aging Time on 2024 Aluminum Behavior
NOTCHES AND THEIR EFFECTS Ali Fatemi - University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations S-N Approach for Notched Members
Compressive (MPa) Setting Time Fineness International Journal of Engineering & Technology IJET-IJENS Vol: 11 No: 04 113 Performance Evaluation of Bamboo Reinforced Concrete Beam M. M. Rahman, M. H. Rashid,
Combusting Candles Category: Chemistry Type: Class Experiment (60 min) Materials List: 2 Tealight candles 1 Nail 1 Glass Jar with a flat top, e.g jam jar 1 Lighter or matches Video: (youtubelink) Be careful!
Mr. Patrick J Camilleri B.Ed (Hons) M.Ed Science (Sheffield) Department of Physics JC Malta Properties of Matter Basics You Should Know Elasticity. Young modulus 1. Hooke's law. Extension α tension (force
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
STRSS-STRAIN RLATIONS Strain Strain is related to change in dimensions and shape of a material. The most elementar definition of strain is when the deformation is along one ais: change in length strain
DEVELOPMENT OF A GRIP AND THERMODYNAMICS SENSITIVE PROCEDURE FOR THE DETERMINATION OF TYRE/ROAD INTERACTION CURVES BASED ON OUTDOOR TEST SESSIONS Flavio Farroni, Aleksandr Sakhnevych, Francesco Timpone
METALLURGY STUDY OF MULTIPHASE MATERIAL USING NANOINDENTATION 3 1 Prepared by Duanjie Li, PhD & Alexis Celestin 6 Morgan, Ste156, Irvine CA 9618 P: 949.461.99 F: 949.461.93 nanovea.com Today's standard
TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INVESTIGATION OF VISCOELASTICITY AND CURE SHRINKAGE IN AN EPOXY RESIN DURING PROCESSING T. Shimizu *, H. Koinuma, K. Nagai Mitsubishi Heavy Industries,
Master's Degree Thesis ISRN: BTH-AMT-EX--2009/D-02--SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
202 Kovove Mater. 43 2005 202 209 EFFECT OF In ADDITION ON Sn-Ag SOLDER, ITS WETTING AND SHEAR STRENGTH OF COPPER JOINTS PAVOL ŠEBO*, PAVOL ŠTEFÁNIK Institute of Materials and Machine Mechanics, Slovak
Numerical Simulation of Temperature and Stress Fields in the Rock Heating Experiment Author P. Rálek 1*, M. Hokr 1 1 Technical University of Liberec, Liberec, Czech Republic *Corresponding author: email@example.com
18th World Conference on Nondestructive Testing, 16-20 April 2012, Durban, South Africa Effects of Various Couplants on Carbon Steel and Aluminium Materials Using Ultrasonic Testing Ngeletshedzo NETSHIDAVHINI
3 rd Year Dental Materials Science Dr. Graham Cross School of Physics and CRANN SFI Nanoscience Building, Rm 1.5 http://www.tcd.ie/physics/people/graham.cross/ Graham.Cross@tcd.ie 16.11.2007 Dental Materials
UDC 624. 042. 7 Development of U-shaped Steel Damper for Seismic Isolation System Kazuaki SUZUKI* 1 Atsushi WATANABE* 1 Eiichiro SAEKI* 1 Abstract Seismic isolation system was widely admitted after Hanshin-Awaji
Materials Transactions, Vol. 53, No. 4 (2012) pp. 604 to 609 Special Issue on APCNDT 2009 2012 The Japanese Society for Non-Destructive Inspection Non-Destructive Evaluation of Weld Structure Using Ultrasonic
Martensite transformation, microsegregation, and creep strength of 9 Cr-1 Mo-V steel weld metal M. L. Santella¹, R. W. Swindeman¹, R. W. Reed¹, and J. M. Tanzosh² ¹ Oak Ridge National Laboratory, Oak Ridge,
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
Recycle of Polyester/Cotton Mixed Yarn as Reinforcement of Hybrid Composite Material Teruo KIMURA, Hiroki HANAMITSU Kyoto Institute of Technology Matsugasaki, Sakyo-ku, Kyoto 66-8585 Japan firstname.lastname@example.org
No.36 (2001) pp.121-126 Synthesis of Large Amount of Pure Negative-Thermal-Expansion Material, ZrW 2 O 8 Takuya HASHIMOTO 1, Tomohiro WAKI 1 and Yuko MORITO 2 (Received September 30, 2000) Abstract The